# Chapter 6: Mechanical Properties

## Presentation on theme: "Chapter 6: Mechanical Properties"— Presentation transcript:

Chapter 6: Mechanical Properties
ISSUES TO ADDRESS... • Stress and strain: What are they and why are they used instead of load and deformation? • Elastic behavior: When loads are small, how much deformation occurs? What materials deform least? • Plastic behavior: At what point does permanent deformation occur? What materials are most resistant to permanent deformation? • Toughness and ductility: What are they and how do we measure them?

Elastic Deformation d F F d 1. Initial 2. Small load 3. Unload

Plastic Deformation (Metals)
1. Initial 2. Small load 3. Unload planes still sheared F d elastic + plastic bonds stretch & planes shear plastic F d linear elastic plastic Plastic means permanent!

Engineering Stress s = F A F t s = A m N or in lb • Tensile stress, s:
original area before loading s = F t A o 2 f m N or in lb Area, Ao • Shear stress, t: Area, Ao F t s = A o  Stress has units: N/m2 or lbf /in2

Common States of Stress
• Simple tension: cable A o = cross sectional area (when unloaded) F o s = F A s Ski lift (photo courtesy P.M. Anderson) • Torsion (a form of shear): drive shaft M A o 2R F s c o t = F s A Note: t = M/AcR here.

OTHER COMMON STRESS STATES (i)
• Simple compression: A o Balanced Rock, Arches National Park (photo courtesy P.M. Anderson) Canyon Bridge, Los Alamos, NM o s = F A Note: compressive structure member (s < 0 here). (photo courtesy P.M. Anderson)

OTHER COMMON STRESS STATES (ii)
• Bi-axial tension: • Hydrostatic compression: Fish under water Pressurized tank (photo courtesy P.M. Anderson) (photo courtesy P.M. Anderson) s z > 0 q s < 0 h

Engineering Strain L w e = d L - d e = w q g = Dx/y = tan
• Tensile strain: d /2 L o w • Lateral strain: e = d L o - d e L = w o d L /2 • Shear strain: q 90º 90º - q y x g = Dx/y = tan Strain is always dimensionless. Adapted from Fig. 6.1(a) and (c), Callister & Rethwisch 8e.

Stress-Strain Testing
• Typical tensile test machine • Typical tensile specimen Adapted from Fig. 6.2, Callister & Rethwisch 8e. gauge length specimen extensometer Adapted from Fig. 6.3, Callister & Rethwisch 8e. (Fig. 6.3 is taken from H.W. Hayden, W.G. Moffatt, and J. Wulff, The Structure and Properties of Materials, Vol. III, Mechanical Behavior, p. 2, John Wiley and Sons, New York, 1965.)

Linear Elastic Properties
• Modulus of Elasticity, E: (also known as Young's modulus) • Hooke's Law: s = E e s Linear- elastic E e F simple tension test

Poisson's ratio, n eL e -n e n = - • Poisson's ratio, n: Units:
metals: n ~ 0.33 ceramics: n ~ 0.25 polymers: n ~ 0.40 Units: E: [GPa] or [psi] n: dimensionless  > density increases  < density decreases (voids form)

Mechanical Properties
Slope of stress strain plot (which is proportional to the elastic modulus) depends on bond strength of metal Adapted from Fig. 6.7, Callister & Rethwisch 8e.

Other Elastic Properties
simple torsion test M t G g • Elastic Shear modulus, G: t = G g • Elastic Bulk modulus, K: pressure test: Init. vol =Vo. Vol chg. = DV P P = - K D V o • Special relations for isotropic materials: 2(1 + n) E G = 3(1 - 2n) K

Young’s Moduli: Comparison
Graphite Ceramics Semicond Metals Alloys Composites /fibers Polymers 0.2 8 0.6 1 Magnesium, Aluminum Platinum Silver, Gold Tantalum Zinc, Ti Steel, Ni Molybdenum G raphite Si crystal Glass - soda Concrete Si nitride Al oxide PC Wood( grain) AFRE( fibers) * CFRE GFRE* Glass fibers only Carbon fibers only A ramid fibers only Epoxy only 0.4 0.8 2 4 6 10 00 1200 Tin Cu alloys Tungsten <100> <111> Si carbide Diamond PTF E HDP LDPE PP Polyester PS PET C FRE( fibers) FRE( fibers)* FRE(|| fibers)* E(GPa) Based on data in Table B.2, Callister & Rethwisch 8e. Composite data based on reinforced epoxy with 60 vol% of aligned carbon (CFRE), aramid (AFRE), or glass (GFRE) fibers. 109 Pa

Useful Linear Elastic Relationships
• Simple tension: • Simple torsion: a = 2 ML o r 4 G M = moment = angle of twist 2ro Lo d = FL o E A d L = - n Fw o E A F A o d /2 L Lo w • Material, geometric, and loading parameters all contribute to deflection. • Larger elastic moduli minimize elastic deflection.

Plastic (Permanent) Deformation
(at lower temperatures, i.e. T < Tmelt/3) • Simple tension test: Elastic+Plastic at larger stress engineering stress, s Elastic initially permanent (plastic) after load is removed ep plastic strain engineering strain, e Adapted from Fig. 6.10(a), Callister & Rethwisch 8e.

Yield Strength, sy y = yield strength sy
• Stress at which noticeable plastic deformation has occurred. when ep = 0.002 tensile stress, s engineering strain, e sy ep = 0.002 y = yield strength Note: for 2 inch sample  = = z/z  z = in Adapted from Fig. 6.10(a), Callister & Rethwisch 8e.

Yield Strength : Comparison
Graphite/ Ceramics/ Semicond Metals/ Alloys Composites/ fibers Polymers Yield strength, s y (MPa) PVC Hard to measure , since in tension, fracture usually occurs before yield. Nylon 6,6 LDPE 70 20 40 60 50 100 10 30 200 300 400 500 600 700 1000 2000 Tin (pure) Al (6061) a ag Cu (71500) hr Ta (pure) Ti Steel (1020) cd (4140) qt (5Al-2.5Sn) W Mo (pure) cw Hard to measure, in ceramic matrix and epoxy matrix composites, since in tension, fracture usually occurs before yield. H DPE PP humid dry PC PET Room temperature values Based on data in Table B.4, Callister & Rethwisch 8e. a = annealed hr = hot rolled ag = aged cd = cold drawn cw = cold worked qt = quenched & tempered

VMSE: Virtual Tensile Testing

Tensile Strength, TS TS engineering stress strain engineering strain
• Maximum stress on engineering stress-strain curve. y strain Typical response of a metal F = fracture or ultimate strength Neck – acts as stress concentrator engineering TS stress engineering strain Adapted from Fig. 6.11, Callister & Rethwisch 8e. • Metals: occurs when noticeable necking starts. • Polymers: occurs when polymer backbone chains are aligned and about to break.

Tensile Strength: Comparison
Si crystal <100> Graphite/ Ceramics/ Semicond Metals/ Alloys Composites/ fibers Polymers Tensile strength, TS (MPa) PVC Nylon 6,6 10 100 200 300 1000 Al (6061) a ag Cu (71500) hr Ta (pure) Ti Steel (1020) (4140) qt (5Al-2.5Sn) W cw L DPE PP PC PET 20 30 40 2000 3000 5000 Graphite Al oxide Concrete Diamond Glass-soda Si nitride H wood ( fiber) wood(|| fiber) 1 GFRE (|| fiber) ( fiber) C FRE A FRE( fiber) E-glass fib Aramid fib Room temperature values Based on data in Table B.4, Callister & Rethwisch 8e. a = annealed hr = hot rolled ag = aged cd = cold drawn cw = cold worked qt = quenched & tempered AFRE, GFRE, & CFRE = aramid, glass, & carbon fiber-reinforced epoxy composites, with 60 vol% fibers.

Ductility x 100 L EL % - = • Plastic tensile strain at failure: Lf Ao
Adapted from Fig. 6.13, Callister & Rethwisch 8e. Engineering tensile strain, e E ngineering tensile stress, s smaller %EL larger %EL Lf Ao Af Lo • Another ductility measure: 100 x A RA % o f - =

Toughness • Energy to break a unit volume of material
• Approximate by the area under the stress-strain curve. very small toughness (unreinforced polymers) Engineering tensile strain, e E ngineering tensile stress, s small toughness (ceramics) large toughness (metals) Adapted from Fig. 6.13, Callister & Rethwisch 8e. Brittle fracture: elastic energy Ductile fracture: elastic + plastic energy

Resilience, Ur 2 1 U e s @ Ability of a material to store energy
Energy stored best in elastic region If we assume a linear stress-strain curve this simplifies to y r 2 1 U e s @ Adapted from Fig. 6.15, Callister & Rethwisch 8e.

Elastic Strain Recovery
syi D syo Elastic strain recovery 2. Unload Stress 1. Load 3. Reapply load Strain Adapted from Fig. 6.17, Callister & Rethwisch 8e.

Hardness • Resistance to permanently indenting the surface.
• Large hardness means: -- resistance to plastic deformation or cracking in compression. -- better wear properties. e.g., 10 mm sphere apply known force measure size of indent after removing load d D Smaller indents mean larger hardness. increasing hardness most plastics brasses Al alloys easy to machine steels file hard cutting tools nitrided diamond

Hardness: Measurement
Rockwell No major sample damage Each scale runs to 130 but only useful in range Minor load kg Major load (A), 100 (B) & 150 (C) kg A = diamond, B = 1/16 in. ball, C = diamond HB = Brinell Hardness TS (psia) = 500 x HB TS (MPa) = 3.45 x HB

Hardness: Measurement
Table 6.5

True Stress & Strain Note: S.A. changes when sample stretched
True strain Adapted from Fig. 6.16, Callister & Rethwisch 8e.

( ) Hardening s e s s • An increase in sy due to plastic deformation.
large hardening s y 1 s y small hardening e • Curve fit to the stress-strain response: s T = K e ( ) n “true” stress (F/A) “true” strain: ln(L/Lo) hardening exponent: n = 0.15 (some steels) to n = 0.5 (some coppers)

Variability in Material Properties
Elastic modulus is material property Critical properties depend largely on sample flaws (defects, etc.). Large sample to sample variability. Statistics Mean Standard Deviation All samples have same value Because of large variability must have safety margin in engineering specifications where n is the number of data points

Design or Safety Factors
• Design uncertainties mean we do not push the limit. • Factor of safety, N Often N is between 1.2 and 4 • Example: Calculate a diameter, d, to ensure that yield does not occur in the 1045 carbon steel rod below. Use a factor of safety of 5. 1045 plain carbon steel: s y = 310 MPa TS = 565 MPa F = 220,000N d L o 5 d = m = 6.7 cm

Summary • Stress and strain: These are size-independent
measures of load and displacement, respectively. • Elastic behavior: This reversible behavior often shows a linear relation between stress and strain. To minimize deformation, select a material with a large elastic modulus (E or G). • Plastic behavior: This permanent deformation behavior occurs when the tensile (or compressive) uniaxial stress reaches sy. • Toughness: The energy needed to break a unit volume of material. • Ductility: The plastic strain at failure.

ANNOUNCEMENTS Reading: Core Problems: Self-help Problems: